Tracking the solid-state incorporation of Sn into the framework of dealuminated zeolite beta, and consequences for catalyst design †

Sn-Beta has emerged as a state-of-the-art catalyst for a range of sustainable chemical transformations. Conventionally prepared by bottom-up hydrothermal synthesis methods, recent research has demonstrated the e ﬃ ciency of several top-down methods of preparation. One attractive top-down approach is Solid-State Incorporation, where a dealuminated Beta zeolite is physically mixed with a solid Sn precursor, in particular Sn( II ) acetate, prior to heat treatment at 550 (cid:1) C. This procedure is fast and benign, and metal incorporation requires no solvents and hence produces no aqueous Sn-containing waste streams. Although the performances of these catalysts have been well explored in recent years, the mechanism of heteroatom incorporation remains unknown, and hence, opportunities to improve the synthetic procedure via a molecular approach remain. Herein, we use a range of in situ spectroscopic techniques, alongside kinetic and computational methods, to elucidate the mechanisms that occur during preparation of the catalyst, and then improve the e ﬃ cacy of the synthetic protocol. Speci ﬁ cally, we ﬁ nd that successful incorporation of Sn into the lattice occurs in several distinct steps, including (i) preliminary coordination of the metal ion to the vacant lattice sites of the zeolite during physical grinding; (ii) partial incorporation of the metal ion into the zeolite framework upon selective decomposition of the acetate ligands, which occurs upon heating the physical mixture in an inert gas ﬂ ow from room temperature to 550 (cid:1) C; and (iii) full isomorphous substitution of Sn into the lattice alongside its simultaneous oxidation to Lewis acidic Sn( IV ), when the physically mixed material is exposed to air during a short (<1 h) isotherm period. Long isotherm steps are shown to be unnecessary, and fully oxidised Sn( IV ) precursors are shown to be unsuitable for successful incorporation into the lattice. We also ﬁ nd that the formation of extra-framework Sn oxides is primarily dependent on the quantity of Sn present in the initial physical mixture. Based on these ﬁ ndings, we demonstrate a faster synthetic protocol for the preparation of Sn-Beta materials via Solid-State Incorporation, and benchmark their catalytic performance for the Meerwein-Ponndorf-Verley transfer hydrogenation reaction and the isomerisation of glucose to fructose.


Introduction
2][3][4][5] In contrast to classical aluminosilicate zeolites, which are widely employed as solid Brønsted acid catalysts, these metallosilicates exhibit high levels of performance as Lewis acid catalysts during liquid phase catalytic reactions.Of particular interest amongst these Lewis acidic metallosilicates is Sn-containing zeolite Beta (Sn-Beta).Sn-Beta is a medium pore BEA-topology zeolite, which contains small amounts of Sn(IV) isomorphously substituted into the otherwise siliceous framework. 60][21][22] Of particular interest are "top-down" methods, in which readily prepared aluminosilicate zeolites are converted into a stannosilicate form by "demetallation-remetallation".In such procedures, a commercially available aluminosilicate is rst dealuminated in HNO 3 , resulting in the formation of silanol nests i.e. vacant "T" sites.3][24][25][26][27] For this reason, dealumination of the parental zeolite is an essential rst step, so that vacant lattice sites are available for subsequent inclusion of a new heteroatom.Amongst top-down approaches, we have demonstrated that solid-state methods of incorporation are particularly suitable. 15,17,28In this approach, heat treatment of a physical mixture of dealuminated zeolite Beta with Sn(OAc) 2 , rstly in nitrogen (N 2 , 3 h) and subsequently in air (3 h), leads to the formation of active Sn-Beta catalysts.This approach, which we have termed Solid-State Incorporation (SSI), possesses several favourable features, including fast synthesis timescales, the absence of solvents and wet chemicals in the remetallation stage, and the ability to incorporate higher loadings of metal than conventional hydrothermal synthesis (>2 wt% Sn). 15,17,28The procedure has also been shown to be amenable for insertion of other metal centres, such as Al(III), Ti(IV) and Zr(IV), when desired. 15,17,24,28,29iven the broad applicability and success of this preparation method, Joshi et al. and Peeters et al. have recently studied the SSI synthesis procedure.In doing so, these groups have determined that the choice of mixing method, and the type of gas employed during the heating step, strongly inuence the eventual speciation and activity of Sn in the nal material. 30,31In particular, Joshi et al. observed that Sn can be directly oxidised to Sn(IV) during the grinding stage if a high energy ball mill is used for mixing. 30On the other hand, Peeters et al. discovered that performing the heat treatment in air ow as opposed to N 2 ow resulted in the formation of both Sn(II) and Sn(IV) species, both of which exhibited different levels of performance for the Baeyer-Villiger oxidation reaction. 31However, although these studies further emphasise how the choice of preparation conditions inuences successful synthesis of the catalyst, they do not directly study the process of heteroatom incorporation at real synthesis conditions, i.e. during the critical stages of the SSI procedure.Hence, limited knowledge is currently available as to what processes occur during conversion of the metal precursor into the nal catalyst.However, such knowledge would make for a powerful tool, since elucidating the mechanism(s) of heteroatom incorporation during SSI could provide a blueprint towards improving the synthesis protocol from a molecular perspective.
By employing state-of-the-art spectroscopic methods, including 119 Sn Carr-Purcell-Meiboom-Gill (CPMG) Magic Angle Spinning (MAS) Nuclear Magnetic Resonance (NMR), in situ X-ray Absorption Spectroscopy (XAS), in situ Diffuse Reectance Infrared Fourier Transform Spectroscopy (DRIFTS), in situ Temperature Programmed Desorption-Mass Spectrometry (TPD-MS), Thermogravimetric analysis, UV-Raman, and Diffuse Reectance UV-Vis (DRUV-Vis) spectroscopy, alongside complimentary kinetic studies and Density Functional Theory (DFT) simulations, we hereby present a detailed study focused upon the chemistry occurring during the synthesis of Sn-Beta catalysts by SSI.In addition to providing unique molecular level insight into the chemical processes occurring during the formation of the Sn-Beta catalyst, this study also reveals which parameters inuence successful synthesis of the catalyst, and thereby reveals how the synthesis protocol can be improved to maximise its rapidity and minimise its energy requirements.The catalytic performances of the materials prepared by the improved synthesis protocol are evaluated by use of the Meerwein-Ponndorf-Verley transfer hydrogenation reaction, and the isomerisation of glucose to fructose at both batch and continuous processing conditions.

Results and discussion
Effect of physical grinding SSI is a two-step procedure (Scheme 1), where dealuminated zeolite Beta and Sn(II) acetate (denoted deAl-Beta and Sn(OAc) 2 , respectively) are rst grinded for 10 min with a pestle and mortar, prior to heat treatment of the solid mixture at elevated temperature (550 C, 3 h in N 2 ow and 3 h in air ow, ramp rate 10 C min À1 ). 15 Prior dealumination of the Beta zeolite is a prerequisite for the synthesis of Sn-Beta by SSI, since the removal of Al from the zeolite generates vacant lattice sites, denoted as silanol nests, the presence of which are required for Sn atoms to eventually be effectively incorporated into the material. 15,22Accordingly, we rst focused on elucidating the changes that occurred to Sn(OAc) 2 during the grinding stage.Although higher Sn content samples are known to possess a greater percentage of spectator sites i.e. extra-framework Sn species, 28,32 a Sn(OAc) 2 /deAl-Beta mixture with a targeted Sn loading of 10 wt% was used for the initial spectroscopic studies, in order to maximise signal to noise ratio and aid spectroscopic denition of the Sn species potentially involved in the incorporation mechanism.Sn-Beta materials possessing higher loadings of Sn (e.g. 10 wt%, denoted 10Sn-Beta) have also been more thoroughly evaluated from a kinetic perspective. 15,17,28,32lthough the physical mixture of Sn(OAc) 2 /deAl-Beta was almost inactive when heat treatment was omitted (ESI Fig. S1 †), changes to the Sn precursor following grinding of the physical mixture were nevertheless evident by 13 C MAS NMR and DRIFT analysis.The 13 C MAS NMR spectrum of untreated Sn(OAc) 2 was composed of two symmetric doublets at À25.6 and À26.7 ppm, and À181.3 and À184.1 ppm (Fig. 1).These doublets correspond to [CH 3 -] and to [C]O], respectively, likely found in two separate crystal environments. 33Although no changes were observed following grinding of the acetate alone, the doublets disappeared when Sn(OAc) 2 was physically mixed with deAl-Beta and only one intense peak for the methyl group, as well as a single, broader carbonyl resonance, were observed.These ndings strongly indicate that grinding Sn(OAc) 2 with the dealuminated zeolite causes its coordination to shi towards monodentate.
Alongside 13 C MAS NMR analysis, DRUV-Vis and DRIFT analysis were also performed.FTIR analysis of the Sn(OAc) 2 / deAl-Beta mixture revealed the formation of a new vibration at 1297 cm À1 upon grinding, and that the difference between the asymmetric and the symmetric stretching modes of C-O, the socalled D value of Sn(OAc) 2 [nCO asym À nCO sym ], 34,35 increased from 187 cm À1 (1600-1413 cm À1 ) in pure Sn(OAc) 2 alone, to 310 cm À1 (1714-1404 cm À1 ) subsequent to grinding with the dealuminated zeolite (Fig. 2a).Physical grinding also modied the Ligand-to-Metal Charge Transfer (LMCT) bands of the Sn precursor, as observed by DRUV-Vis (Fig. 2b).The physically mixed sample Sn(OAc) 2 /deAl-Beta lost the lower energy signal at 245 nm associated with pure Sn(OAc) 2 .Notably, none of the changes to the D value or LMCT bands were observed when Sn(OAc) 2 was grinded alone i.e. when the dealuminated zeolite material was absent (ESI Fig. S2-S3 †), suggesting that the presence of the dealuminated zeolite is required for these changes to occur.
5][36] A shi towards monodentate coordination is further supported by detection of an additional vibrational feature at 1297 cm À1 for the Sn(OAc) 2 /deAl-Beta mixture, which has been attributed to monodentate acetate groups. 34Further support to this hypothesis was provided by computational analysis, which predicts that the D value of Sn(OAc) 2 [nCO asym À nCO sym ] 35 increases from 102 cm À1 to 307 cm À1 when comparing pure Sn(OAc) 2 and Sn(OAc) 2 /deAl-Beta, respectively (ESI Fig. S4 †).
To investigate the role of the silanol nests produced during the dealumination process, and determine how these particular vacant sites are involved in the change of coordination of the acetate ligands, a control sample was prepared by grinding Sn(OAc) 2 with Si-Beta, which is a purely siliceous sample of zeolite beta that has not undergone dealumination.Although Si-Beta possesses external silanol groups, it does not possess the internal T-atom vacancies surrounded by four Si-OH groups (i.e.silanol nests), as found in dealuminated zeolite Beta, which are formed by removal of the original aluminium centres.
Grinding Sn(OAc) 2 with a sample of Si-Beta also increases the D value, and generates the feature at 1297 cm À1 , indicating that any silanol functionality can facilitate the change in acetate coordination.However, the spectral changes observed were somewhat more extensive for the deAl-Beta mixture, and the 1297 cm À1 feature was clearly of lower intensity when deAl-Beta was replaced by Si-Beta, both of which indicate that greater change occurs when internal silanol nests are present alongside the external silanol groups (ESI Fig. S5 and S6 †).
To elucidate the impact of the grinding step on the Sn centres, preliminary XAS measurements were performed on the Sn(OAc) 2 /deAl-Beta grinded mixture and important reference samples (ESI Fig. S7 †).Despite the changes exhibited by the acetate ligands during physical mixing, Sn was still found to be tetrahedral in geometry and in the +2 oxidation state in the grinded mixture, indicating that the overall speciation of the metal did not change during physical grinding.This suggests that, upon grinding, partial coordination of Sn to the zeolite occurred without change in oxidation state, with the lattice providing two of the bonds required to maintain tetrahedral geometry aer the change in acetate coordination from bidentate to monodentate.The XAS data is more deeply discussed in the following section.
Further indications of metal-zeolite interactions aer physical grinding were provided by UV-Raman analysis.Upon grinding, new bands in the region of 550-650 cm À1 were observed, the presence of which have previously been attributed to Sn-O vibrations (Fig. 3). 37Notably, the intensity of these bands was found to depend on the quantity of Sn mixed with the dealuminated zeolite, i.e. the intensity of the new bands increased going from 2 wt% of Sn to 10 wt%, whilst none of these vibrations was observed when grinding Sn(OAc) 2 alone.Moreover, the bands observed between 550-650 cm À1 remained present even aer heat treatment and removal of the acetate ligand (ESI Fig. S8 †).Consequently, these bands can reasonably be assigned to Sn-O bonds in a range of different congurations as a result of interactions between Sn(OAc) 2 and the zeolite. 37g. 3 UV-Raman spectra of (i) deAl-Beta (black line), (ii) pure Sn(OAc) 2 (red line), and Sn(OAc) 2 /deAl-Beta mixture with (iii) 2 wt% of Sn (blue line), and iv) 10 wt% of Sn (green line).In summary, spectroscopic study of the rst step of the SSI procedure revealed that, upon grinding the metal precursor with deAl-Beta, the acetate precursor switched from a bridged bidentate coordination to a more monodentate one.However, these changes were not accompanied by changes to the Sn centres, which remained in the oxidation state +2 and in a tetrahedral geometry, due to partial coordination to the zeolite.Comparison with control samples also showed different Sn(OAc) 2 -zeolite interactions occurred in the presence of silanol nests (i.e.substituting Si-Beta with deAl-Beta).These ndings contrast to those recently reported by Joshi et al., which indicated formation of Sn(IV) via mechanochemical grinding using a high energy ball mill, as opposed to physical grinding. 30evertheless, samples of Sn(OAc) 2 /deAl-Beta, Sn(OAc) 2 /Si-Beta, and SnO 2 /deAl-Beta exhibited null or negligible levels of catalytic activity (ESI Fig. S1 †), 15,28 demonstrating that the heat treatment step typically employed during SSI is essential to generate catalytic properties.
Evolution of Sn during heat treatment of Sn(OAc) 2 /deAl-Beta Despite the changes that occur to Sn(OAc) 2 during the grinding stage, poor catalytic activity was observed for the Sn(OAc) 2 /deAl-Beta grinded mixture (ESI Fig. S1 †).Thus, to obtain substantial catalytic activity by SSI, heat treatment of Sn(OAc) 2 /deAl-Beta is clearly required.During previous research, the heat treatment has been performed by heating the sample to 550 C (10 C min À1 ), rst in a ow of N 2 (ramp and 3 h isotherm), and subsequently in a ow of air (3 h), at gas ow rates of 60 mL min À1 throughout for 1.5 g of catalyst (WHSV ¼ $2400 h À1 ). 28ccordingly, to understand how the physically grinded 'precatalyst' gains catalytic activity, the evolution of the metal precursor/deAl-Beta mixture during heat treatment was followed at real conditions with a variety of in situ techniques, including TPD-MS, DRIFTS and XAS.Control experiments were also performed on grinded samples of Sn(OAc) 2 alone, deAl-Beta alone, and a physical mixture of Sn(OAc) 2 /Si-Beta, where required.Also in this case, spectroscopic studies were rst focused using 10 wt% of Sn, to favour spectral denition, although specic experiments were later repeated for catalysts containing lower loadings of Sn to provide additional molecular insights (1 wt%, vide infra).
To better understand the nature of the interactions between Sn(OAc) 2 and the zeolite, the gaseous effluent generated during various heat treatments was monitored by Mass Spectrometry (TPD-MS) (Fig. 4).To maximise rigour, the MS system was connected directly to the calcination furnace employed for conventional catalyst synthesis, and identical conditions were used to our standard protocol.Furthermore, tracer experiments performed with CaCO 3 were conducted to determine the delay between the evolution of the compound and the detection of the MS, and all reported spectra were offset accordingly (ESI Fig. S9 †).To determine the relevance of the effluent evolutions with respect to formation of an active catalyst, control experiments were performed by measuring the gaseous effluent generated from Sn(OAc) 2 alone, and a Sn(OAc) 2 /Si-Beta mixture, which did not result in the production of an active catalyst.For clarity, the ramping stage and the N 2 /air switch stage of the heat treatment are expanded in Fig. 4, as no changes were observed in the intermediate isotherms.However, the full TPD-MS proles are presented for completion in SI Fig. S10-S12, † alongside the TPD-MS prole of deAl-Beta alone (ESI Fig. S13 †).
In the absence of any zeolite material, pure Sn(OAc) 2 decomposes at temperatures #280 C, primarily releasing CO 2 , alongside smaller quantities of acetone and trace quantities of acetic acid.In contrast, TPD-MS of the Sn(OAc) 2 /Si-Beta mixture resulted rst into evolution of acetic acid and CO 2 at temperatures <250 C, followed by the formation of acetone and additional CO 2 in the temperature range 250-400 C. The observations suggest that the co-presence of Si-Beta, and/or residual water molecules present in the siliceous zeolite, induces hydrolysis of the acetate precursor prior to its full decomposition.The observation is in line with the known hydrolysis and decomposition behaviour of acetate compounds. 38,39n contrast, mixing Sn(OAc) 2 with deAl-Beta drastically modies the decomposition process, shiing all product evolutions to a higher temperatures range (350-550 C) compared to the temperatures found in the two former cases (<400 C).Specically, two intense peaks related to acetone and CO 2 were observed at ca. 435 C, while small amounts of acetic acid were gradually decomposed throughout the ramping period.The detection of volatile compounds at higher temperatures ($350 C) for the Sn(OAc) 2 /deAl-Beta mixture clearly indicates that stronger Sn(OAc) 2 -zeolite interactions occur when silanol nests are present.Interestingly, the TPD-MS prole of a deAl-Beta sample previously impregnated with acetic acid revealed similar product evolution to the Sn(OAc) 2 /deAl-Beta mixture (ESI Fig. S14 †), suggesting that primary interconversion of the acetate ligands into acetic acid, prior to further decomposition into CO 2 , may be a key step towards the synthesis of an active catalyst.We note that no volatile products were detected during the initial isotherm period for any physical mixture, and that only small traces of CO 2 were evolved Fig. 5 TGA profiles and derivatives of (from top to bottom) (i) pure Sn(OAc) 2 , (ii) Sn(OAc) 2 /Si-Beta, and (iii) Sn(OAc) 2 /deAl-Beta.
when the inert gas was switched to air aer the rst 3 h isotherm period (Fig. 4b).
Complementing the TPD-MS data, the mass loss proles of these samples were also measured by TGA during the initial ramping stage (Fig. 5).The mass loss proles of both Sn(OAc) 2 and Sn(OAc) 2 /Si-Beta are in excellent agreement to the TPD-MS data, exhibiting one major mass loss between 100-300 C. Interestingly, the total mass lost during treatment of pure Sn(OAc) 2 does not fully account for all the acetate present in the sample (mass loss of 40%, in contrast to approximately 50% mass of acetate in Sn(OAc) 2 ).Since no further decomposition occurred during the isotherm (Fig. 4), the observation suggests that a solid product of higher mass than elemental Sn was formed, i.e. an oxide, carbonate, or oxycarbonate product.On the other hand, the mass loss prole of Sn(OAc) 2 /deAl-Beta exhibited mass losses up to 500 C, in which the loss of mass observed at low temperatures (<200 C) can be attributed to (partial) dehydration of deAl-Beta.
The ndings from TPD-MS and TGA clearly indicate that the rate and mechanism of acetate decomposition is strongly inuenced by the presence of a zeolite.Also, these changes were not solely due to additional hydrolysis processes caused by the presence of water present in the hydrated zeolite, since the pathway of acetate decomposition is different for Sn(OAc) 2 /Si-Beta and Sn(OAc) 2 /deAl-Beta.Hence, the mechanism is particularly modied when the zeolite also possesses silanol nests.These ndings are in good agreement with the FTIR spectra reported in ESI Fig. S5 and S6, † which revealed different interactions occurring between Sn(OAc) 2 /deAl-Beta and Sn(OAc) 2 /Si-Beta.
To gain further insights into the various mechanisms occurring during heat treatment, in situ DRIFTS measurements were subsequently performed.DRIFT analysis of Sn(OAc) 2 /deAl-Beta (Fig. 6) revealed various changes to the 1755-1200 cm À1 region upon heating the sample to 325 C, which may be related to changes in the acetate coordination and/or dehydration of the zeolite.Control experiments using Sn(OAc) 2 alone (ESI Fig. S15 †) and deAl-Beta alone (ESI Fig. S16 †) conrmed that changes in intensity at 1751, 1714 (nCO asym ), 1541 (nCO asym ), 1413 (nCO sym ) and 1280 cm À1 only occurred for the Sn(OAc) 2 / deAl-Beta physical mixture, suggesting these rearrangements to be related to changes in acetate coordination in the presence of the zeolite.As the temperature further increased from 325 C to 550 C, all the CO stretching bands disappeared, suggesting total decomposition of the acetate ligands.The result is in good agreement with the TPD-MS and TGA analysis.Due to the dehydration processes that occur throughout the heating step, a decrease in vOH bands located in the region 3750-3250 cm À1 was also observed.This nding is in agreement with 29 Si MAS NMR analysis performed on samples of Sn(OAc) 2 /deAl-Beta removed from the furnace aer different periods of time during the ramping stage.Specically, 29 Si MAS NMR analysis revealed that the signal at À98 ppm, assigned to isolated (Si(-OSi-) 3 OH) groups (Q 3 ), [40][41][42] decreased in the temperature range 300-550 C (ESI Fig. S17 †), suggesting a reduction in defect sites during heat treatment of the physical mixture.In situ DRIFT analysis of the following stages of the heat treatment was also performed, indicating that only minor changes occurred throughout the three hours isotherm in N 2 and the three hours isotherm in air, whilst re-hydration of the material was clearly observed at the end of the calcination (ESI Fig. S18 †).
To complement these ndings and gain further insight into the changes occurring to the Sn species in the sample, the evolution of Sn during heat treatment was followed by in situ Xray Absorption Spectroscopy (XAS).This experiment was performed using a Sn(OAc) 2 /deAl-Beta mixture with 10 wt% Sn, whose nal form obtained aer heat treatment is denoted as 10Sn-Beta.It is also worth noting that although the beamline could only provide helium (He) rather than N 2 as inert gas, reference experiments (spectroscopic and catalytic) performed on 10Sn-Beta prepared in He/air demonstrated that precisely the same catalytic activity was observed for samples prepared in He/air and N 2 /air, for the Meerwein-Ponndorf-Verley (MPV) transfer hydrogenation of cyclohexanone to cyclohexanol (ESI Fig. S19-S21 and Table S1 Firstly, changes within the near edge structure by X-ray Absorption Near Edge Structure (XANES) were investigated by examining the maximum of the rst derivative of the XANES data.Grinding Sn(OAc) 2 with deAl-Beta led to a slight shi in edge position, although this was still consistent with Sn(II) being overwhelmingly present following physical grinding (ESI Fig. S7 †).Heat treatment of the sample under the X-ray beam was subsequently performed at the precise conditions typically employed by SSI, albeit with He used instead of N 2 as inert gas.
To aid the understanding of the changes in the XANES spectra, the position of the 1 st derivative maxima were plotted against time, allowing the oxidation state of Sn during the heat treatment to be monitored.4][45][46] During the rst stages of the heat treatment (ramp to 550 C and 3 h isotherm in He ow), very little change was observed to the oxidation state of Sn, with Sn(II) clearly still present throughout the rst isotherm in inert gas (Fig. 7a).However, signicant changes to the XANES spectrum occurred upon switching the gas stream from the inert carrier to air (Fig. 7a).The introduction of air led to extremely rapid increases in the oxidation state of Sn.Indeed, within 60 min, the oxidation state of Sn increased from +2 to +4.
To gain further insight on how these changes correlate to the structure of the catalyst, and in particular the coordination environment of Sn, Extended X-ray Absorption Fine Structure (EXAFS) measurements were also performed (Fig. 7b, Tables 1 and ESI Table S2 †).To simplify interpretation and the level of analysis required, focus was placed on the speciation of Sn (i) in the Sn(OAc) 2 /deAl-Beta mixture (i.e.prior heat treatment) and, (ii) just prior to, and following, the switch to air, where the major spectral changes were expected based on XANES.Firstly, Sn(OAc) 2 was tted to that expected from its crystal structure using two Sn-O paths at distances of 2.161 AE 0.013 Å (rst-shell Sn-O) and 2.885 AE 0.024 Å (second-shell Sn-O) with coordination numbers of 4 and 3, respectively.Notably, the latter path arises from interactions between distinct [SnO 4 ] centres, which is indicative of a crystalline material.Upon grinding Sn(OAc) 2 with deAl-Beta, a reduction in the rst-shell path length from 2.161 AE 0.013 Å to 2.087 AE 0.015 Å was observed (Table 1 entries 1 and 2), supporting the proposed changes in coordination of the acetate groups suggested by DRIFT and 13 C MAS NMR analysis (Fig. 1 and 2).This change was also accompanied by the disappearance of the second-shell Sn-O path length at 2.885 AE 0.024 Å, indicating loss of the long-range order found in pure Sn(OAc) 2 , and conrming dispersion of the Sn centres on the zeolite (Table 1 entries 1 and 2).Moreover, a coordination number of 4.2 was measured, supporting the hypothesis that,   Upon cooling the sample following the heat treatment, a higher coordination number (ca.4.8) was observed.This is consistent with facile rehydration of the catalyst upon cooling, in line with our previous EXAFS studies of hydrated Sn-Beta catalysts. 28s previously mentioned, Sn-Beta catalysts with high Sn loadings also possess unwanted spectator Sn species, which do not contribute to the catalytic activity of the material.To investigate the rate and extent of formation of these sites, focus was placed on both Sn-O and Sn-Sn scattering during the oxidation step (Fig. 8, presenting the magnitude of the k 3weighted Fourier transform of the EXAFS spectrum of the mixture in R-space).The rst features present in the spectra (1-2 Å) in Fig. 8 can be assigned to Sn-O scattering interactions, whilst Sn-Sn scattering indicative of clustered/extra-lattice Sn species can be identied by features between 3.0 and 4 Å. 45 Prior to the introduction of air, only one major feature is observed at approximately 1.8 Å, indicative of Sn-O bonding.Upon introduction of air into the system, a signicant increase in the intensity of the rst peak in the FT spectrum occurred, indicating either (i) an increase in the number of Sn-O bonds, (ii) an increase in the order and uniformity of the existing Sn-O bonds, or (iii) a combination of both.
Furthermore, upon switching to air, the feature at approximately 3.2 Å increases at a similar rate to that at 1.8 Å.The increase in the feature at $3.2 Å throughout the heat treatment protocol indicates some Sn-Sn formation occurs regardless of how long the heat treatment protocol is carried out for at these Sn loadings.Although preliminary, this observation suggests that both framework and extra-framework Sn species are formed at the same period of time, at this metal loading with this Sn precursor, albeit to different absolute quantities.This suggests that formation of Sn-Sn species may be related to the spatial proximity of Sn, and may not be possible to control by kinetic means.
Further elucidation of Sn incorporation into the zeolite lattice was achieved by 119 Sn CPMG MAS NMR spectroscopy, performed in direct excitation (DE) mode. 47Technical limitations prohibited analysis of the samples at true operational conditions, and hence, the heat treatment was terminated at various stages prior to  removal of the sample and measurement by ex situ 119 Sn MAS NMR.0][51][52][53] 119 Sn MAS NMR spectra of Sn(OAc) 2 /deAl-Beta obtained at different stages of the ramp only revealed minimal changes, showing À600 ppm species to still be the dominant resonance (Fig. 9).Moreover, no changes were observed throughout the rst isotherm step (N 2 ow), in excellent agreement with the XAS analysis.Upon switching the gas ow to air, changes in Sn speciation were evident, with a prominent increase in intensity at À689 ppm, which can be readily attributed to the active Sn species based on several previous reports (Fig. 9). 32,42,54Notably, only minor changes to the À689 ppm signal were detected over the nal two hours in air, supporting the XAS analysis and indicating that isomorphous substitution occurs during the rst stages of the air isotherm, when the oxidation state of Sn increases from +2 to +4.Due to the fact a variety of Sn-O compounds, including Sn(OAc) 2 , generate resonances at À600 ppm (ESI Fig. S24 †), 17 it is difficult to say from 119 Sn MAS NMR analysis at which stage extra-framework Sn species form.Still, the nal 119 Sn MAS NMR spectrum strongly resembles those well benchmarked for active Sn-Beta samples prepared with higher loadings of Sn i.e. >5 wt%, which are known to contain a mixed active site population of isomorphously substituted Sn and extra-framework Sn compounds.Taken together, the XANES, EXAFS and 119 Sn MAS DE CPMG NMR analyses all indicate that full isomorphous substitution of Sn into the framework of zeolite Beta, and its oxidation to Lewis acidic Sn(IV), only occurs upon introduction of air into the system.These ndings are in line with those reported by Peeters et al. 31 who, by means of 119 Sn Mössbauer Spectroscopy, found that a Sn(IV)/Sn(II) ratio of 95/5 was obtained when Sn-Beta was heated rst in a N 2 ow followed by air ow, whilst only 18% of Sn(IV) was formed when heating Sn-Beta in N 2 only, i.e. in the absence of air.

Increasing the relative proportion of active sites; spectroscopic analysis of 1Sn-Beta
As we have previously demonstrated, 17,28 Sn-Beta catalysts possessing initial Sn loadings >5 wt% typically contain higher quantities of extra-framework SnO x species than Sn-Beta catalysts possessing Sn loadings of #2 wt%.Although these species do not contribute to the catalytic performance of the material, they can evidently inuence the spectroscopic signals generated, which may complicate mechanistic understanding of this system.Accordingly, key experiments described above were repeated for samples of 1Sn-Beta, containing only 1 wt% Sn, which were also synthesised by SSI of a Sn(OAc) 2 /deAl-Beta mixture.Although samples with lower metal loadings are oen more challenging to characterise due to their lower levels of signal to noise, studying samples with a higher fraction of active to inactive sites evidently allows better evaluation of which of the processes occurring during SSI are most relevant to catalysis and active site formation.We note that our recent studies of continuous glucose to fructose isomerisation have revealed that the turnover frequency of Sn is approximately 7fold higher in 1Sn-Beta than for 10Sn-Beta. 17,28,32irstly, DRIFT measurements were performed on Sn(OAc) 2 / deAl-Beta (nal Sn loading of 1 wt%) prior to heat treatment, revealing similar changes in the acetate coordination to the ones observed for the high loading sample (ESI Fig. S25 †).However, in situ DRIFT analysis performed throughout the ramping stage (Fig. 10a, and ESI Fig. S26 † for full spectra) indicated a greater level of clarity present in the 1% Sn mixture when compared to the high loading analogue.Specically, upon heating the 1% Sn mixture, rapid decrease of the CO asym stretching band at 1709 cm À1 was observed, accompanied by the formation of a band at 1751 cm À1 at 125 C, which then disappeared at 375 C.These ndings clearly indicate changes of C]O coordination throughout the ramp, prior to full decomposition of the acetate groups at temperatures >325 C. The formation of a band at 1751 cm À1 because of a changing acetate ligand is supported by DFT vibrational analysis, which reveals a similar shi to a higher frequency (D ¼ 40 cm À1 ) when a proton moves from the zeolite framework to the acetate ligand, yielding free acetic acid (ESI Fig. S27 †).Moving to the following stages of the heat treatment, no change was observed throughout the isotherm in N 2 , whilst minor changes were observed in the isotherm in air in the -OH region (3750-3250 cm À1 ).Notably, fast rehydration of the catalyst was again observed upon cooling the sample to room temperature following synthesis, suggesting the formation of hydrated Sn sites (Fig. 10b).Summarising, DRIFT analysis of the 1 wt% Sn sample is in good agreement with that of the high loading analogue, conrming initial changes in acetate coordination in the temperature range 25-325 C, likely related to the initial formation of acetic acid, which further decomposed at temperatures >325 C.
Further key experiments repeated on 1Sn-Beta revealed that the major changes in both acetate evolution and Sn speciation previously observed for 10Sn-Beta were all comparable for 1Sn-Beta, suggesting that they were all broadly relevant to the synthesis of active Sn species.In particular, 29 Si-and 119 Sn-MAS NMR (ESI Fig. S28 and S29 †), along with TPD-MS (ESI Fig. S30 †), were shown to be consistent with the results obtained from 10Sn-Beta.However, a much smaller relative fraction of acetone was observed in the TPD-MS spectrum of 1Sn-Beta when compared to that of 10Sn-Beta.The negligible quantity of acetone in this case appears to correlate with the lower quantity of extra-framework Sn species formed at lower Sn loadings.DRIFT analysis of 1Sn-Beta presented minor differences due to the better resolution of 1Sn-Beta, showing clear formation of acetic acid and conrming the key role that it has during the synthesis of an active catalyst.

Proposed mechanism
Coupling both experimental and computational data, several observations on the mechanism that controls the incorporation of Sn into the zeolite lattice may be deduced.Focusing on the rst step of SSI, i.e. physical mixing of Sn(OAc) 2 with deAl-Beta, the following conclusions can be made: (i) Sn retains its oxidation state of +2 and a tetrahedral geometry (XAS and 119 Sn MAS NMR), (ii) the acetate groups change their coordination to gain a more monodentate character ( 13 C NMR and DRIFT), (iii) different acetate-zeolite interactions can be observed when silanol nests are present (DRIFT and TPD-MS), and (iv) direct interactions between Sn and the zeolite lattice are observed (DRIFT, EXAFS, Raman), and must occur in order to maintain tetracoordinated Sn species despite the monodentate nature of the acetates following grinding.Despite the complicated network of hydrogen bonds established between Sn(OAc) 2 and molecules of water and/or silanol sites, a simplied scheme for the grinding step is proposed in Scheme 2. It should be noted that at this particular stage of preparation, the material exhibits very low levels of catalytic activity (ESI Fig. S1 †).
To gain substantial catalytic activity, heat treatment of the physical mixture Sn(OAc) 2 /deAl-Beta is required (550 C, 3 h N 2 and 3 h air).Based on the spectroscopic data obtained, the ramping stage and the rst hour of isotherm in air are the key steps to achieve Sn incorporation.Throughout the ramping stage it was found that: (i) most of the acetate is released at temperatures higher than 325 C (TPD-MS), (ii) CO 2 , acetone and acetic acid are the main products detected (TPD-MS), although acetic acid is clearly the primary product (TPD-MS, DRIFTS and DFT analysis), (iii) most of the Sn centres retain an oxidation state of +2 (XAS) and form tetracoordinated species ( 119 Sn MAS DE CPMG NMR, XAS).
Focusing on the subsequent key step, i.e. moving from N 2 to air, the following observations can be made: (i) Sn is rapidly oxidised from +2 to +4 (XANES), (ii) a large percentage of Sn centres are subjected to a change of coordination, and become consistent with Sn atoms that are isomorphously substituted into the Beta lattice (EXAFS and 119 Sn MAS DE CPMG NMR), (iii) concurrently to the formation of framework Sn centres, some Sn-Sn interactions, indicative of extra-framework Sn species, are observed (EXAFS) and (iv) the nal catalyst samples reveal a large percentage of the À689/À703 ppm species which are associated with hydrated active species ( 119 Sn MAS DE CPMG NMR). 28,29hese ndings indicate that several chemical processes are clearly relevant during SSI.Throughout the ramping stage (Scheme 3), partial coordination of Sn in the zeolite, i.e.
Scheme 2 Proposed species formed throughout the grinding step.formation of the rst Sn-O-Si bonds, may be achieved by donation of a proton from an adjacent silanol site to the acetate group, resulting in formation of free acetic acid (TPD-MS and DRIFT).Transition state calculations with DFT predict the formation of acetic acid from a monodentate acetate-Sn species, and its subsequent dissociation, are relatively low energy (#0.72 eV), suggesting that the production of acetic acid would be facile from the initial physically mixed state of the catalyst (ESI Fig. S31 †).Though the reaction is endothermic, entropic contributions can likely drive the process forward.Further decomposition of free acetic acid likely accounts for the generation of the majority of the products detected in the gas effluent of Sn(OAc) 2 /deAl-Beta (TPD-MS).This conclusion is supported by a TPD-MS experiment performed on a sample of deAl-Beta previously impregnated with acetic acid (ESI Fig. S14 †), which results in the generation of a gaseous effluent comparable to the standard preparation procedure, with CO 2 detected as main product alongside smaller amounts of acetic acid, acetone, and hydrogen.Based on the observations made for 10Sn-Beta, and especially the analogous experiments performed on 1Sn-Beta, we conclude this to be the preliminary step required to eventually form active, isomorphously-substituted Sn(IV) atoms.
Alongside this route, reaction pathways involving the release of acetone (TPD-MS) can also occur.Considering that higher percentages of acetone are observed at higher loadings of Sn, we propose that acetone could be formed from two neighbouring acetate groups.Based on steric reasons, we hypothesise that interactions between two proximal acetate groups may provide the opportunity for acetone to be released.Although interactions among proximal Sn acetate centres may be considered negligible in mixtures with low Sn loading (i.e. 1 wt%), such a mechanism may easily occur on materials with Sn loading $5 wt%, which are known to lead to Sn-Beta catalysts with higher percentages of extra-framework Sn, and, thus, more spectator Sn species. 13,14This effect is in excellent agreement with the much higher percentage of acetone detected during TPD-MS of Sn(OAc) 2 /deAl-Beta mixture with 10% Sn, compared to its low loading analogue (1 wt% Sn, ESI Fig. S30 †), which exhibited only traces of acetone, and which is known to possess only small quantities of extra-framework Sn. 17,32 Changing the calcination gas to the highly oxidising conditions, in addition to the presence of water vapour found in compressed air, leads to the genesis of Sn centres with the oxidation state +4, at the same time that XAS studies indicate full incorporation of Sn into the lattice occurs.To determine the full relationship between the oxidation state increase and full incorporation into the lattice, a series of experiments were performed using Sn(OAc) 4 as precursor.Although use of this precursor resulted in a similar grinded complex being formed between Sn(OAc) 4 /deAl-Beta as found for Sn(OAc) 2 /deAl-Beta (ESI Fig. S32 †), the Sn(OAc) 4 /deAl-Beta mixture was inactive when tested for the MPV reaction (SI Fig. S33 †).The inactivity indicates that full isomorphous substitution of Sn into the zeolite lattice is essential for the synthesis of an active Sn-Beta catalyst, and not simply coordination of a Sn(IV) containing precursor.Furthermore, the Sn-Beta material prepared following heat treatment of Sn(OAc) 4 /deAl-Beta still exhibited poor activity for the MPV reaction when compared to the conventional Sn-Beta analogue prepared with Sn(OAc) 2 (ESI Fig. S33 †).This suggests full isomorphous substitution of Sn into the lattice cannot occur when a Sn(IV) precursor is used.Taken together, these results indicate that although Sn(OAc) 4 and deAl-Beta interact in a similar manner to Sn(OAc) 2 and deAl-Beta, Sn(II) is required to prepare a Sn-Beta material with substantial catalytic performances (ESI Fig. S33 †).The nding also suggests that oxidation of Sn from +2 to +4 is undesirable during the grinding stage, and should preferentially occur throughout the heat treatment.This nding likely explains why poorer catalytic performance is achieved when a high energy ball mill is used for preparation, since such instruments have been shown to cause oxidation of Sn from +2 to +4 prior to heat treatment, potentially hindering isomorphous substitution.
On another level, however, these ndings also suggest that full isomorphous substitution cannot be achieved if there is no oxidative driving force, strongly indicating that the oxidation and incorporation events are linked.Based on this, we propose that Sn oxidation occurs via hydrogen abstraction from Sn-O(H)-Si to Sn-O-Si bonds (Scheme 3), which leads to concurrent oxidation of Sn(II) to Sn(IV) whilst simultaneously achieving full incorporation of Sn(IV) species into the zeolite lattice.Transition state modelling indicates that direct release of H 2 from geminal -SiOH bonds (Scheme 3) is characterised by a kinetic barrier of 3.26 eV, but a drastic reduction in the kinetic barrier to 1.38 eV occurs when transferring hydrogen via water (ESI Fig. S34 †).The reduced barrier suggests that a network of water molecules, which may be present in the pore, but also in compressed air, would aid in the transfer of hydrogen during the oxidation step.Finally, hydration of Sn-Beta readily occurs throughout the cooling step, leading to the genesis of hydrated Sn sites, which are characterised by NMR signals at À689/ À703 ppm.In regards to the formation of extra-framework Sn species, XAS studies indicate that their formation occurs at the same time as isomorphous substitution of Sn into the lattice, albeit to a lower absolute degree.This suggests that the ratio of active sites/spectator sites cannot be controlled by kinetic means, and instead depends on the spatial distribution of Sn, since the relative fraction of these undesirable species is much lower for samples with lower Sn loadings.Based on the TPD-MS experiments performed for 10Sn-Beta and 1Sn-Beta, we hypothesize that extra-framework Sn formation occurs due to the competing formation of acetone from two neighboring acetate groups, the probability of which increases markedly at higher loadings of Sn.

Application of mechanistic insight
In addition to providing detailed mechanistic insight regarding the reactions occurring during the synthesis of Sn-Beta catalysts by SSI, the in situ spectroscopic data presented above suggests that long stages of the SSI synthesis procedure are superuous to form active Sn-Beta catalysts.To clarify whether the extended stages of both isotherms were unnecessary with respect to forming active Sn-Beta catalysts, and with the objective of streamlining the synthesis procedure for future optimisation studies in mind, a nal series of experiments aimed at clarifying the unnecessary nature of the isotherm periods was performed.Despite possessing higher distribution of spectator sites compared to 1Sn-Beta, 10Sn-Beta was used as the material for this study for two reasons.Firstly, its higher loading results in improved productivity per gram of catalyst, making it a more interesting material from an industrial perspective.Secondly, its higher ratio of spectator sites/active sites provides greater opportunity for improved catalyst performance, if extraframework Sn species can be avoided simply by shortening the synthesis procedure.Based on spectroscopic data, two important key points were determined to be essential to synthesise an active catalyst: (i) the use of a N 2 ramp, and (ii) subsequent change to air ow to oxidise the Sn(II) to Sn(IV).Therefore, to experimentally determine whether the long isotherm steps were superuous, a new 10Sn-Beta material was prepared as follows: a physical mixture of Sn(OAc) 2 and deAl-Beta was heated to 550 C in a ow of N 2 at a ramp rate of 10 C min À1 , before N 2 ow was switched to a ow of air once a temperature of 550 C was achieved.The furnace was subsequently held at 550 C for one hour in air ow.The catalyst prepared with the rapid calcination is henceforth denoted as 10Sn-Beta (0 h, 1 h), whilst the conventional sample synthesised using three hours isotherm in N 2 and three hours isotherm in air, is denoted as 10Sn-Beta (3 h, 3 h).The catalytic performances of both samples were then investigated for batch MPV reaction of cyclohexanone to cyclohexanol using 2-butanol as a secondary alcohol, and for the isomerisation of glucose to fructose, which are two reactions prevalent for the testing of Sn-Beta catalysts. 8,9,54-579][60][61] To compare the intrinsic activity of the catalysts, turnover frequency (TOF) values were calculated during the early stage of batch reactions using eqn (4) in the Experimental Section, and reported in Fig. 11.When comparing the catalyst prepared with the shortened synthesis procedure to the conventional one, similar TOF values were observed for both MPV and glucose isomerisation reactions.Specically, both catalysts exhibited TOFs of 200 AE 20 h À1 for MPV reaction of cyclohexanol to cyclohexanone, whilst TOFs of 17 h À1 and 14 h À1 were achieved on both catalysts for glucose conversion and fructose yield, respectively.The essentially identical values observed in Fig. 11 conrm identical catalytic performances between the conventional catalyst and the more rapidly prepared catalysts.This demonstrates that the successful synthesis of 10Sn-Beta can be achieved even with removal of the superuous isotherm stages, conrming that isomorphous substitution of Sn by SSI remains successful even if the heat treatment protocol is shortened by 5 h.
To verify whether the shortened synthesis procedure affected the stability of the isomorphously substituted Sn, additional glucose isomerisation experiments were performed at continuous processing conditions (Fig. 12).In line with the batch reactivity data, negligible differences to the TOF value of 10Sn-Beta were observed, despite the 5 h reduction of synthesis time.Moreover, at the conditions explored, the rate of deactivation (k d ) of Sn-Beta catalyst was almost unaffected by the rapid preparation method, presenting a k d of 0.13 h À1 (0 h, 1 h) in contrast to 0.10 h À1 obtained from the original procedure (3 h, 3 h) (ESI Fig. S35 †).Details on Levenspiel plots for rate of deactivation can be found in SI Fig. S35.† Thus, it is clear that omitting the isotherm step in N 2 and reducing the time in air by 67% resulted in no loss in performance compared to the original material.Although the relationship between Sn species and TOF is nontrivial, 18 with even different framework sites displaying different TOF values, 32 we note that the fact the TOF values did not increase following the rapid synthesis procedure suggests that the formation of extra-framework Sn species is not avoided simply by shortening the synthesis procedure.This provides further conrmation that the formation of extra-framework Sn species is determined by the spatial distribution of Sn acetate, and not by the agglomeration of isomorphously substituted Sn(IV) atoms during the extended heat treatment protocol.

Conclusions
Using a broad range of in situ and ex situ techniques, along with computational simulations, this study investigated the key steps for the successful incorporation of Sn into the lattice of dealuminated Beta (deAl-Beta) zeolite by Solid State Incorporation.Spectroscopic analysis of the conventional synthetic protocol allowed us to gain insights into the key mechanistic steps, and then apply these ndings to improve the synthesis procedure of Sn-Beta.We identied that although Sn does not fully incorporate into the lattice upon physical mixing alone, interactions between the Sn(OAc) 2 precursor and the dealuminated zeolite occurred during this stage of the preparation, resulting in coordination of the acetate to the vacant lattice sites of the zeolite matrix.Subsequent heating of the Sn(OAc) 2 /deAl-Beta mixture to 550 C under inert gas ow (N 2 or He) is required to remove the acetates from Sn(OAc) 2 , and achieve the rst stages of Sn incorporation.However, this step alone is insufficient to synthesise highly active Sn-Beta catalysts, and we nd that replacing the inert gas ow with air ow at high temperatures is required to oxidise the Sn species from an oxidation state of +2 to +4, which occurs simultaneous to the full incorporation of Sn in the lattice.Formation of the active site, proposed to be a Sn(IV) species resonating at À689 ppm by 119 Sn MAS NMR spectroscopy, and typically assigned to hydrated Sn centres, occurs during the rst hour from the introduction of air in the calcination furnace, indicating completion of the synthesis during this time.Alongside Sn incorporation, XAS analysis revealed that spectator species such as SnO 2 are formed at the same time that Sn is incorporated into the lattice, suggesting that the active species/ spectator species ratios are driven by proximity of Sn centres, and are not controlled by kinetic means.Based on these mechanistic ndings, we demonstrate that successful preparation of Sn-Beta can be achieved in a total of only two hours, by shortening the synthesis procedure so that it only includes the rst ramp in N 2 , and the rst hour of isotherm in air.Catalytic analysis of Sn-Beta materials prepared by this streamlined synthesis procedure, for the Meerwein-Pondorf-Verley transfer hydrogenation reaction of cyclohexanone to cyclohexanol and the isomerisation of glucose to fructose, reveal identical performance between the conventional Sn-Beta catalyst and that prepared by our shorter heat treatment method.Along with providing a more rapid procedure for future optimisation studies, this also demonstrates how the mechanistic information generated by in situ spectroscopic analysis can be used to make practical improvements to the Sn-Beta synthesis procedure.Kinetic studies MPV reactions.Batch reactions for the MPV reduction using cyclohexanone and 2-butanol as the secondary alcohol were performed in a 50 mL round bottom ask equipped with a reux condenser, controlled thermostatically by being immersed in a silicon oil bath.The vessel was charged with a 10 mL solution of cyclohexanone in 2-butanol (0.2 M) with biphenyl (0.01 M) used as the internal standard.The ask was subsequently heated to the desired temperature (100 C internal temperature).An aliquot prior to the addition of the catalyst was obtained and analysed to obtain the initial point (t 0 ) by immersing and letting the vessel reach internal temperature.The reaction started when Sn-Beta catalyst (1 mol% of Sn relative to cyclohexanone) was added to the ask, which was then stirred at AE750 rpm.Aliquots were taken periodically from the ask, centrifuged and subsequently analyzed in a GC-FID (Agilent 7820, 25m CP-Wax 52 CB).

Experimental section
Glucose isomerisation reactions.Batch D-glucose (Sigma-Aldrich, 99%) isomerisation experiments were performed in 15 mL thick-walled glass reactors (Ace pressure tube, Sigma-Aldrich) that were heated in a temperature-controlled oil bath.The reactor was charged with 5 mL of an aqueous solution of glucose (1 wt% in MeOH) and an appropriate amount of catalyst corresponding to a 1 : 50 metal:glucose molar ratio.Once the oil had reached the desired temperature (110 C), the reaction commenced with vigorous stirring with a magnetic stirrer bar (750 rpm).The reactor was stirred for an appropriate length of time, and time online samples were obtained by periodically quenching the reaction by rapidly cooling the reactor in an ice bath.Aliquots of solution were extracted with a syringe, centrifuged to remove solid particulates, and were subsequently analysed by 1260 Innity HPLC coupled with a Hi-Plex Ca (6.5 Â 300 mm, 8m particle size, Agilent) column, which was isothermally held at 80 C, and an ELS detector where sorbitol was used as an external standard.HPLC grade water was used as the mobile phase, at a ow rate of 0.75 mL min À1 .
Continuous D-glucose isomerisation was performed in a plug ow, tubular (1/4 00 , 4.1 mm ID) stainless-steel reactor using 1 wt% glucose in MeOH as feed.The reactor was connected to an HPLC pump to regulate the reactant ow and be able to operate in high pressures.Catalysts (100 mg) were placed between two plugs of quartz wool and packed in the reactor with a 0.5 mm frit in the reactor outlet.The reactor was then immersed in a thermostatic oil bath at 110 C. Pressure in the system was controlled using a backpressure regulator, set at the desired pressure (typically 10 bar).Experiments were performed with a ow rate of 1 mL min À1 .Periodic aliquots were taken from the reactor outlet and analysed by an Agilent 1260 Innity HPLC coupled with a Hi-Plex Ca column and an ELS detector, where sorbitol was used as an external standard.

Formulas and mathematical expressions
Levenspiel rate of deactivation :

Catalyst characterization
Specic surface area (SSA) was determined from N 2 adsorption using the BET equation, and microporous volume was determined from N 2 adsorption isotherms using the t-plot method.Porosimetry measurements were performed on a Quantachrome Quadrasorb, and samples were degassed prior to use (300 C, 12 h).Adsorption isotherms were obtained at 77 K. TGA analysis was performed on a PerkinElmer system.Samples were held isothermally at 30 C for 30 min before being heated to 550 C (10 C min À1 ramp rate) in N 2 .TPD-MS measurements were performed on a homemade system formed by a mass ow controllers (MFC) equipped with a horizontal tube furnace where the sample is placed, connected with a Hiden QGA Mass Spectrometer.A weighed amount of catalyst was placed inside a calcination boat and placed in the horizontal furnace and compound evolutions were monitored by the aforementioned spectrometer.The furnace was heated from 30 to 550 C (ramp rate 10 C min À1 ) and a constant ow of N 2 was used throughout the experiment (20 mL min À1 ).N 2 ow was switched to air aer reaching set temperature and continued for 1 h.
Nuclear Magnetic Resonance (NMR) was carried out in a Bruker Avance III HD 400 MHz NMR spectrometer. 119Sn, 1 H, 13 C and 29 Si NMR were carried out at operating frequencies of 149.23, 400.20, 188.41 and 79.508 MHz, respectively.All analyses were run with a 10 kHz spin rate, with samples packed into ZrO 2 rotors. 119Sn MAS DE CPMG NMR experiments were performed with the CPMG echo-train acquisition as described in ref. 47 and 49.Spectra were measured by applying 100 echoes, using a 2.5 ms 90 -pulse with a 180 proton decoupling.The relaxation delay (t 1 ) was set to 5 s, and 2048 scans were performed.Sn chemical shis were calibrated using Sn(IV) oxide as reference. 29Si MAS NMR were obtained by one-pulse experiment with a 4 ms 45 -pulse with a 20 seconds recycle delay and 128 scans.Chemical shis were calibrated using the Si(0Al) ( 4 Q) chemical shi at À110 ppm of the commercial aluminium Beta zeolite. 62,63 1H MAS NMR were obtained by a one-pulse experiment with a 2.5 ms pulse with a 3 seconds recycle delay.Adamantane was used for calibration of the 1 H chemical shis. 13C CP MAS were acquired with a relaxation delay of t 1 ¼ 5 s, using 2048 scans where glycine was used as the reference of 13 C chemical shi.
DRIFT spectroscopy analyses were performed in a Harrick praying mantis cell, using a Bruker Tensor II spectrometer over a range of 4000-650 cm À1 at a resolution of 2 cm À1 .In situ DRIFT spectroscopy was performed with the same conditions under ow.The samples were heated at a ramp rate of 10 C min À1 to set temperature 550 C under N 2 ow, held at 550 C under N 2 ow for 3 h, then switched to air ow (20 mL min À1 ) for another 3 h.Raman spectra were obtained with a Renishaw inVia spectrometer equipped with a laser line at 266 nm.UV-Vis analysis was performed using a Cary 4000 UV-Vis spectrophotometer.The scan range was done between 200-800 at a scan rate of 200 nm min À1 .

Computational simulation
Density functional theory (DFT) calculations were performed using the numeric atomic orbital (NAO) package, FHI-aims, which is an all-electron, full-potential electronic code structure, and is suitable for periodic and non-periodic systems. 64The generalised gradient approximation exchangecorrelation functional of Perdew, Burke and Ernzerhof, reparameterised for solids (PBEsol), was used; several density functionals were tested, with PBEsol chosen due to its good comparative performance, and acceptance within the computational community. 65Dispersion interactions were accounted for using the Tkatchenko-Scheffler method, which is a pair-wise additive approach to include van der Waals interactions within the simulation. 66Calculations were performed using a 'light' basis set (version: 2010), with self-consistent eld (SCF) convergence reached when the charge density was 10 À6 e/a 0 3 .
Calculations were performed spin-restricted throughout, and the ZORA approximation was applied to provide relativistic treatments. 67ructure optimisation, vibrational simulations and transition state sampling An initial BEA unit cell structure was obtained from the International Zeolite Association (IZA) database. 68Models were built and manipulated using the Atomic Simulation Environment (ASE) python library. 69Full geometry and unit cell optimisations were performed on all structures using the Broyden-Fletcher-Goldfarb-Shanno (BFGS) algorithm, [70][71][72][73] with convergence reached when the residual forces on all atoms were less than 0.01 eV ÅÀ1 .Optimisations were performed with a converged Monkhorst-Pack 74 k-grid (2 Â 2 Â 2).Vibrational frequencies were also calculated on optimised structures using ASE, and scaled by a parameterised factor 75 of 0.99 to correct for systematic over approximations, allowing direct comparison with experiment.
Transition state structures and minimum energy pathways were identied using a machine learning nudged elastic band (ML-NEB) method approached, implemented in the CatLearn soware. 76This machine learning approach uses a Gaussian process regression to evaluate uncertainty estimates of all images in a reaction pathway and sets this uncertainty to be a criterion for convergence.To improve computational efficiency without compromising accuracy, atoms beyond a distance from 2 nearest neighbours from the reaction site were frozen.Convergence was assumed when the force on individual atoms was below 0.05 eV ÅÀ1 and the average uncertainty in the interpolated pathway was below 0.05 eV.

X-ray Absorption Spectroscopy analysis
Sn K-edge XAFS studies were performed on the B18 beamline at Diamond Light Source, Didcot, UK, using a Si(111) double crystal monochromator and were measured in transmission mode.The samples were placed into a Harrick X-ray transmission DRIFTS cell, details of which have been described previously. 77,78Spectra were recorded over 2 min intervals (k max ¼ 14, step size 0.5 eV), and on average three scans were acquired to improve the signal-to-noise level of the data for transmission measurements of each spectrum.All XAFS spectra were acquired concurrently with the appropriate foil placed between I t and I ref .XAFS data processing was performed using IFEFFIT 79 with the Horae package 80 (Athena and Artemis).The amplitude reduction factor was derived from EXAFS data analysis of two reference compounds, SnO 2 , (with known coordination numbers which were xed during analysis) to be 1.0, which was used as a xed input parameter, and Sn(OAc) 2 .

Scheme 1
Scheme 1 Schematic of the Solid-State Incorporation (SSI) procedure.

Fig. 4
Fig. 4 TPD-MS during calcination of (from top to bottom) (i) Sn(OAc) 2 /deAl-Beta, (ii) Sn(OAc) 2 /Si-Beta, and iii) pure Sn(OAc) 2 .(a) TPD-MS plots of the first 2 hours which includes the initial ramp from room temperature to 550 C and part of the N 2 isotherm.(b) TPD-MS plots of the N 2 /air switch step, following the 3 h isotherm in N 2 at 550 C.

Fig. 7
Fig. 7 In situ XAS analysis of 10Sn-Beta synthesis.(a) Oxidation state of Sn as a function of time.(b) Coordination number of Sn and first-shell Sn-O bond distance obtained from XANES fitting data (further details are reported in ESITable S2 †).
upon grinding, the majority of the Sn atoms remain tetrahedrally coordinated.Upon heating the Sn(OAc) 2 /deAl-Beta to 550 C under inert atmosphere, a stable coordination number of Sn equal to +3.3 AE 0.5 with a Sn-O distance of 2.04 AE 0.02 Å was observed (Fig.7b), revealing a reduction in both coordination number of Sn and rst-shell Sn-O path length, relative to the freshly ground sample.Upon changing the inert gas ow to air, signicant changes to the material undergoing heat treatment were observed.Firstly, a notable reduction in 2s 2 was observed (from 0.0125 AE 0.0031 Å2 in He ow, to 0.0075 AE 0.0019 Å2 aer 16 min in air ow), suggesting an increase in the order of the local environment.Furthermore, within 16 min aer switching to air ow, the Sn coordination number increased from ca. 3.4 to 4, and the Sn-O path length was reduced to a value of 1.956 AE 0.012 Å. Notably, these values for the rst-shell Sn-O bond distance are consistent with that of Sn atoms that are isomorphously substituted into the Beta framework, 46 conrming that full isomorphous substitution occurs at the same time as the Sn atoms are oxidised from 2 to 4. Throughout this stage, the Sn atoms remain tetrahedrally coordinated, characterised by a Sn coordination number of 4 and an Sn-O bond distance of 1.956 Å, due to their dehydrated nature at high temperatures.

Fig. 8
Fig. 8 EXAFS 3D spectrum of the k 3 weighted FT of 10Sn-Beta calcination in R-space.

Fig. 9
Fig. 9 119 Sn MAS DE CPMG NMR spectra of 10Sn-Beta at different stages of the ramping period in N 2 , and at different stages of the isotherm periods.

Fig. 10
Fig. 10 DRIFT spectra during heat treatment of Sn(OAc) 2 /deAl-Beta mixture with 1 wt% of Sn (a) at different moments of the ramping stage in N 2 (zoom on CO asym bands) and (b) different steps of the isotherms and cooling to room temperature.

Scheme 3
Scheme 3 Proposed steps for the insertion of Sn into the zeolite lattice.(a) Simplified scheme for the acetate removal, forming a tetrahedral Sn(II) species.(b) Oxidation step occurring in air at 550 C, where Sn(IV) is obtained by loss of 2 hydrogen atoms.(c) Simplified scheme for the hydration of the fully incorporated Sn(IV) centres, occurring during the cooling stage from 550 C to room temperature in air.We note that X corresponds to either a Si atom or an H atom arising from hydrolysis of the Sn-O-Si bond, which would also result in the generation of a neighbouring silanol site.
Catalyst synthesisA commercial zeolite Al-b (Zeolyst, NH 4 + -form, Si/Al ¼ 38) was dealuminated by treatment in HNO 3 solution (13 M HNO 3 , 100 C, 20 mL g À1 zeolite, 20 h).Solid-state stannation of dealuminated zeolite b was performed according to the procedure reported in ref.17, by grinding the appropriate amount of Sn(OAc) 2 with the necessary amount of dealuminated zeolite for 10 min in a pestle and mortar.Following this procedure, the samples were heated in a combustion furnace (Carbolite MTF12/38/400) to 550 C with a ramp rate of 10 C min À1 , rst in a ow of N 2 and subsequently changed to air (60 mL min À1 ) aer reaching set temperature and desired isotherm time.

Table 1
EXAFS fitting data of selected stages of the catalyst during synthesis of Sn-Beta a a Fitting parameters: S 0 2 ¼ 1 as deduced by SnO 2 and Sn(OAc) 2 standard; Fit range 2.5 < k< 13, 1 < R < 4; Number of independent points ¼ 19.Values in parenthesis give the experimental error.